#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/90/4509031.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_4509031
loop_
_publ_author_name
'Xue, Liping'
'Wang, Yongjing'
'Lv, Peiwen'
'Chen, Dagui'
'Lin, Zhang'
'Liang, Jingkui'
'Huang, Feng'
'Xie, Zhi'
_publ_section_title
;
 Growth, Structures, and Properties of Li2Zn2(MoO4)3and Co-doped
 Li2Zn2(MoO4)3
;
_journal_issue                   2
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              914
_journal_paper_doi               10.1021/cg800700h
_journal_volume                  9
_journal_year                    2009
_chemical_formula_sum            'Co0.19 Li0.93 Mo1.5 O6 Zn0.88'
_chemical_formula_weight         315.36
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   5.0869(10)
_cell_length_b                   10.533(2)
_cell_length_c                   17.686(4)
_cell_measurement_temperature    293(2)
_cell_volume                     947.6(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0142
_diffrn_reflns_av_sigmaI/netI    0.0229
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            2031
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         2.25
_exptl_absorpt_coefficient_mu    8.983
_exptl_absorpt_correction_T_max  0.4986
_exptl_absorpt_correction_T_min  0.3880
_exptl_crystal_density_diffrn    4.421
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1164
_exptl_crystal_size_max          0.13
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.09
_refine_diff_density_max         1.026
_refine_diff_density_min         -1.388
_refine_diff_density_rms         0.213
_refine_ls_extinction_coef       0.0087(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.039
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     104
_refine_ls_number_reflns         1150
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0267
_refine_ls_R_factor_gt           0.0236
_refine_ls_shift/su_max          0.050
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0637P)²+6.4362P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0861
_refine_ls_wR_factor_ref         0.0943
_reflns_number_gt                1075
_reflns_number_total             1150
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg800700hsup1.cif
_cod_data_source_block           a
_cod_original_formula_sum        'Co0.19 Li0.93 Mo1.50 O6 Zn0.88'
_cod_database_code               4509031
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 1.22156(4) 0.2500 0.556499(13) 0.00772(5) Uani 1 2 d S
Mo2 Mo 0.27699(3) 0.027130(16) 0.343692(9) 0.00877(4) Uani 1 1 d .
Zn1 Zn 0.75427(6) 0.07756(3) 0.471500(19) 0.00787(9) Uani 0.6168(8) 1 d P
Li1 Li 0.75427(6) 0.07756(3) 0.471500(19) 0.00787(9) Uani 0.352(4) 1 d P
Co1 Co 0.75427(6) 0.07756(3) 0.471500(19) 0.00787(9) Uani 0.0282(10) 1 d P
Zn2 Zn 0.6077(2) -0.2500 0.25072(4) 0.0304(2) Uani 0.3992(11) 2 d SP
Li2 Li 0.6077(2) -0.2500 0.25072(4) 0.0304(2) Uani 0.451(4) 2 d SP
Co2 Co 0.6077(2) -0.2500 0.25072(4) 0.0304(2) Uani 0.1504(14) 2 d SP
Zn3 Zn 0.7453(3) 0.2500 0.30233(9) 0.0291(4) Uani 0.1331(14) 2 d SP
Li3 Li 0.7453(3) 0.2500 0.30233(9) 0.0291(4) Uani 0.693(4) 2 d SP
Co3 Co 0.7453(3) 0.2500 0.30233(9) 0.0291(4) Uani 0.1775(17) 2 d SP
O1 O 1.1374(4) 0.2500 0.65264(11) 0.0155(5) Uani 1 2 d S
O2 O 1.4198(3) 0.11590(14) 0.53719(8) 0.0123(3) Uani 1 1 d .
O3 O 0.9424(4) 0.2500 0.49294(11) 0.0118(4) Uani 1 2 d S
O4 O 0.5608(3) 0.11425(14) 0.37276(8) 0.0143(3) Uani 1 1 d .
O5 O 0.0818(3) -0.01035(14) 0.42466(8) 0.0134(3) Uani 1 1 d .
O6 O 0.0789(3) 0.12418(15) 0.28678(8) 0.0176(4) Uani 1 1 d .
O7 O 0.3581(3) -0.11412(14) 0.29563(8) 0.0149(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Mo1 O2 109.05(6) . 7_565
O1 Mo1 O2 109.05(6) . .
O2 Mo1 O2 106.00(9) 7_565 .
O1 Mo1 O3 114.23(10) . .
O2 Mo1 O3 109.09(6) 7_565 .
O2 Mo1 O3 109.09(6) . .
O1 Mo1 Li1 105.19(6) . 7_565
O2 Mo1 Li1 83.38(5) 7_565 7_565
O2 Mo1 Li1 138.70(5) . 7_565
O3 Mo1 Li1 33.345(14) . 7_565
O6 Mo2 O7 110.48(7) . .
O6 Mo2 O4 109.29(7) . .
O7 Mo2 O4 112.54(7) . .
O6 Mo2 O5 105.64(7) . .
O7 Mo2 O5 109.28(7) . .
O4 Mo2 O5 109.39(6) . .
O4 Zn1 O5 97.46(6) . 1_655
O4 Zn1 O3 102.22(7) . .
O5 Zn1 O3 95.31(7) 1_655 .
O4 Zn1 O2 92.65(6) . 1_455
O5 Zn1 O2 162.93(6) 1_655 1_455
O3 Zn1 O2 95.95(7) . 1_455
O4 Zn1 O5 170.30(6) . 5_656
O5 Zn1 O5 83.23(6) 1_655 5_656
O3 Zn1 O5 87.32(7) . 5_656
O2 Zn1 O5 84.52(6) 1_455 5_656
O4 Zn1 O2 85.56(6) . 5_756
O5 Zn1 O2 83.31(6) 1_655 5_756
O3 Zn1 O2 172.22(6) . 5_756
O2 Zn1 O2 83.80(6) 1_455 5_756
O5 Zn1 O2 84.92(5) 5_656 5_756
O4 Zn1 Li1 138.94(4) . 5_756
O5 Zn1 Li1 42.33(4) 1_655 5_756
O3 Zn1 Li1 91.68(5) . 5_756
O2 Zn1 Li1 124.44(4) 1_455 5_756
O5 Zn1 Li1 40.90(4) 5_656 5_756
O2 Zn1 Li1 82.13(4) 5_756 5_756
O4 Zn1 Zn1 138.94(4) . 5_756
O5 Zn1 Zn1 42.33(4) 1_655 5_756
O3 Zn1 Zn1 91.68(5) . 5_756
O2 Zn1 Zn1 124.44(4) 1_455 5_756
O5 Zn1 Zn1 40.90(4) 5_656 5_756
O2 Zn1 Zn1 82.13(4) 5_756 5_756
Li1 Zn1 Zn1 0.000(16) 5_756 5_756
O4 Zn1 Li1 88.66(4) . 5_656
O5 Zn1 Li1 122.86(5) 1_655 5_656
O3 Zn1 Li1 138.81(6) . 5_656
O2 Zn1 Li1 43.41(4) 1_455 5_656
O5 Zn1 Li1 82.90(4) 5_656 5_656
O2 Zn1 Li1 40.39(4) 5_756 5_656
Li1 Zn1 Li1 105.90(2) 5_756 5_656
Zn1 Zn1 Li1 105.90(2) 5_756 5_656
O7 Zn2 O7 87.40(9) . 7
O7 Zn2 O7 92.92(7) . 6_656
O7 Zn2 O7 179.37(4) 7 6_656
O7 Zn2 O7 179.37(4) . 4_545
O7 Zn2 O7 92.92(7) 7 4_545
O7 Zn2 O7 86.75(9) 6_656 4_545
O7 Zn2 O1 87.34(7) . 2_654
O7 Zn2 O1 87.34(7) 7 2_654
O7 Zn2 O1 92.13(6) 6_656 2_654
O7 Zn2 O1 92.13(6) 4_545 2_654
O7 Zn2 O1 93.73(6) . 5_756
O7 Zn2 O1 93.73(6) 7 5_756
O7 Zn2 O1 86.79(7) 6_656 5_756
O7 Zn2 O1 86.79(7) 4_545 5_756
O1 Zn2 O1 178.52(11) 2_654 5_756
O7 Zn2 Zn2 128.08(5) . 6_656
O7 Zn2 Zn2 128.08(5) 7 6_656
O7 Zn2 Zn2 52.04(5) 6_656 6_656
O7 Zn2 Zn2 52.04(5) 4_545 6_656
O1 Zn2 Zn2 125.13(7) 2_654 6_656
O1 Zn2 Zn2 53.39(7) 5_756 6_656
O7 Zn2 Co2 128.08(5) . 6_656
O7 Zn2 Co2 128.08(5) 7 6_656
O7 Zn2 Co2 52.04(5) 6_656 6_656
O7 Zn2 Co2 52.04(5) 4_545 6_656
O1 Zn2 Co2 125.13(7) 2_654 6_656
O1 Zn2 Co2 53.39(7) 5_756 6_656
Zn2 Zn2 Co2 0.00(3) 6_656 6_656
O7 Zn2 Li2 128.08(5) . 6_656
O7 Zn2 Li2 128.08(5) 7 6_656
O7 Zn2 Li2 52.04(5) 6_656 6_656
O7 Zn2 Li2 52.04(5) 4_545 6_656
O1 Zn2 Li2 125.13(7) 2_654 6_656
O1 Zn2 Li2 53.39(7) 5_756 6_656
Zn2 Zn2 Li2 0.00(3) 6_656 6_656
Co2 Zn2 Li2 0.00(3) 6_656 6_656
O7 Zn2 Li2 52.48(5) . 6_556
O7 Zn2 Li2 52.48(5) 7 6_556
O7 Zn2 Li2 127.39(5) 6_656 6_556
O7 Zn2 Li2 127.39(5) 4_545 6_556
O1 Zn2 Li2 53.72(7) 2_654 6_556
O1 Zn2 Li2 127.76(7) 5_756 6_556
Zn2 Zn2 Li2 178.85(6) 6_656 6_556
Co2 Zn2 Li2 178.85(6) 6_656 6_556
Li2 Zn2 Li2 178.85(6) 6_656 6_556
O7 Zn2 Co2 52.48(5) . 6_556
O7 Zn2 Co2 52.48(5) 7 6_556
O7 Zn2 Co2 127.39(5) 6_656 6_556
O7 Zn2 Co2 127.39(5) 4_545 6_556
O1 Zn2 Co2 53.72(7) 2_654 6_556
O1 Zn2 Co2 127.76(7) 5_756 6_556
Zn2 Zn2 Co2 178.85(6) 6_656 6_556
Co2 Zn2 Co2 178.85(6) 6_656 6_556
Li2 Zn2 Co2 178.85(6) 6_656 6_556
Li2 Zn2 Co2 0.00(3) 6_556 6_556
O7 Zn2 Zn2 52.48(5) . 6_556
O7 Zn2 Zn2 52.48(5) 7 6_556
O7 Zn2 Zn2 127.39(5) 6_656 6_556
O7 Zn2 Zn2 127.39(5) 4_545 6_556
O1 Zn2 Zn2 53.72(7) 2_654 6_556
O1 Zn2 Zn2 127.76(7) 5_756 6_556
Zn2 Zn2 Zn2 178.85(6) 6_656 6_556
Co2 Zn2 Zn2 178.85(6) 6_656 6_556
Li2 Zn2 Zn2 178.85(6) 6_656 6_556
Li2 Zn2 Zn2 0.00(3) 6_556 6_556
Co2 Zn2 Zn2 0.00(3) 6_556 6_556
O4 Zn3 O4 85.03(10) . 7_565
O4 Zn3 O6 146.50(9) . 7_665
O4 Zn3 O6 90.50(6) 7_565 7_665
O4 Zn3 O6 90.50(6) . 1_655
O4 Zn3 O6 146.50(9) 7_565 1_655
O6 Zn3 O6 75.26(10) 7_665 1_655
O4 Zn3 O6 81.13(6) . 6_656
O4 Zn3 O6 130.57(8) 7_565 6_656
O6 Zn3 O6 124.82(8) 7_665 6_656
O6 Zn3 O6 81.04(6) 1_655 6_656
O4 Zn3 O6 130.57(8) . 4
O4 Zn3 O6 81.13(6) 7_565 4
O6 Zn3 O6 81.04(6) 7_665 4
O6 Zn3 O6 124.82(8) 1_655 4
O6 Zn3 O6 73.06(9) 6_656 4
O4 Zn3 Zn3 89.30(5) . 6_556
O4 Zn3 Zn3 89.30(5) 7_565 6_556
O6 Zn3 Zn3 123.89(8) 7_665 6_556
O6 Zn3 Zn3 123.89(8) 1_655 6_556
O6 Zn3 Zn3 43.62(6) 6_656 6_556
O6 Zn3 Zn3 43.62(6) 4 6_556
O4 Zn3 Li3 89.30(5) . 6_556
O4 Zn3 Li3 89.30(5) 7_565 6_556
O6 Zn3 Li3 123.89(8) 7_665 6_556
O6 Zn3 Li3 123.89(8) 1_655 6_556
O6 Zn3 Li3 43.62(6) 6_656 6_556
O6 Zn3 Li3 43.62(6) 4 6_556
Zn3 Zn3 Li3 0.00(3) 6_556 6_556
O4 Zn3 Li3 134.83(5) . 6_656
O4 Zn3 Li3 134.83(5) 7_565 6_656
O6 Zn3 Li3 45.04(4) 7_665 6_656
O6 Zn3 Li3 45.04(4) 1_655 6_656
O6 Zn3 Li3 83.73(7) 6_656 6_656
O6 Zn3 Li3 83.73(7) 4 6_656
Zn3 Zn3 Li3 107.91(9) 6_556 6_656
Li3 Zn3 Li3 107.91(9) 6_556 6_656
O4 Zn3 Zn3 134.83(5) . 6_656
O4 Zn3 Zn3 134.83(5) 7_565 6_656
O6 Zn3 Zn3 45.04(4) 7_665 6_656
O6 Zn3 Zn3 45.04(4) 1_655 6_656
O6 Zn3 Zn3 83.73(7) 6_656 6_656
O6 Zn3 Zn3 83.73(7) 4 6_656
Zn3 Zn3 Zn3 107.91(9) 6_556 6_656
Li3 Zn3 Zn3 107.91(9) 6_556 6_656
Li3 Zn3 Zn3 0.00(5) 6_656 6_656
Mo1 O1 Co2 158.43(13) . 2_655
Mo1 O1 Li2 158.43(13) . 2_655
Co2 O1 Li2 0.00(5) 2_655 2_655
Mo1 O1 Zn2 158.43(13) . 2_655
Co2 O1 Zn2 0.00(5) 2_655 2_655
Li2 O1 Zn2 0.00(5) 2_655 2_655
Mo1 O1 Zn2 128.68(12) . 5_756
Co2 O1 Zn2 72.89(6) 2_655 5_756
Li2 O1 Zn2 72.89(6) 2_655 5_756
Zn2 O1 Zn2 72.89(6) 2_655 5_756
Mo1 O1 Li2 128.68(12) . 5_756
Co2 O1 Li2 72.89(6) 2_655 5_756
Li2 O1 Li2 72.89(6) 2_655 5_756
Zn2 O1 Li2 72.89(6) 2_655 5_756
Zn2 O1 Li2 0.00(2) 5_756 5_756
Mo1 O1 Co2 128.68(12) . 5_756
Co2 O1 Co2 72.89(6) 2_655 5_756
Li2 O1 Co2 72.89(6) 2_655 5_756
Zn2 O1 Co2 72.89(6) 2_655 5_756
Zn2 O1 Co2 0.00(2) 5_756 5_756
Li2 O1 Co2 0.00(2) 5_756 5_756
Mo1 O2 Co1 136.25(8) . 1_655
Mo1 O2 Zn1 136.25(8) . 1_655
Co1 O2 Zn1 0.00(2) 1_655 1_655
Mo1 O2 Li1 136.25(8) . 1_655
Co1 O2 Li1 0.00(2) 1_655 1_655
Zn1 O2 Li1 0.00(2) 1_655 1_655
Mo1 O2 Co1 121.16(7) . 5_756
Co1 O2 Co1 96.20(6) 1_655 5_756
Zn1 O2 Co1 96.20(6) 1_655 5_756
Li1 O2 Co1 96.20(6) 1_655 5_756
Mo1 O2 Li1 121.16(7) . 5_756
Co1 O2 Li1 96.20(6) 1_655 5_756
Zn1 O2 Li1 96.20(6) 1_655 5_756
Li1 O2 Li1 96.20(6) 1_655 5_756
Co1 O2 Li1 0.000(14) 5_756 5_756
Mo1 O2 Zn1 121.16(7) . 5_756
Co1 O2 Zn1 96.20(6) 1_655 5_756
Zn1 O2 Zn1 96.20(6) 1_655 5_756
Li1 O2 Zn1 96.20(6) 1_655 5_756
Co1 O2 Zn1 0.000(14) 5_756 5_756
Li1 O2 Zn1 0.000(14) 5_756 5_756
Mo1 O3 Zn1 118.17(5) . .
Mo1 O3 Co1 118.17(5) . 7_565
Zn1 O3 Co1 120.92(10) . 7_565
Mo1 O3 Zn1 118.17(5) . 7_565
Zn1 O3 Zn1 120.92(10) . 7_565
Co1 O3 Zn1 0.00(2) 7_565 7_565
Mo1 O3 Li1 118.17(5) . 7_565
Zn1 O3 Li1 120.92(10) . 7_565
Co1 O3 Li1 0.00(2) 7_565 7_565
Zn1 O3 Li1 0.00(2) 7_565 7_565
Mo2 O4 Zn1 122.59(8) . .
Mo2 O4 Zn3 122.43(8) . .
Zn1 O4 Zn3 114.69(8) . .
Mo2 O5 Co1 131.80(8) . 1_455
Mo2 O5 Zn1 131.80(8) . 1_455
Co1 O5 Zn1 0.00(2) 1_455 1_455
Mo2 O5 Li1 131.80(8) . 1_455
Co1 O5 Li1 0.00(2) 1_455 1_455
Zn1 O5 Li1 0.00(2) 1_455 1_455
Mo2 O5 Co1 123.03(8) . 5_656
Co1 O5 Co1 96.77(6) 1_455 5_656
Zn1 O5 Co1 96.77(6) 1_455 5_656
Li1 O5 Co1 96.77(6) 1_455 5_656
Mo2 O5 Li1 123.03(8) . 5_656
Co1 O5 Li1 96.77(6) 1_455 5_656
Zn1 O5 Li1 96.77(6) 1_455 5_656
Li1 O5 Li1 96.77(6) 1_455 5_656
Co1 O5 Li1 0.00(2) 5_656 5_656
Mo2 O5 Zn1 123.03(8) . 5_656
Co1 O5 Zn1 96.77(6) 1_455 5_656
Zn1 O5 Zn1 96.77(6) 1_455 5_656
Li1 O5 Zn1 96.77(6) 1_455 5_656
Co1 O5 Zn1 0.00(2) 5_656 5_656
Li1 O5 Zn1 0.00(2) 5_656 5_656
Mo2 O6 Co3 137.11(9) . 1_455
Mo2 O6 Zn3 137.11(9) . 1_455
Co3 O6 Zn3 0.00(9) 1_455 1_455
Mo2 O6 Li3 137.11(9) . 1_455
Co3 O6 Li3 0.00(9) 1_455 1_455
Zn3 O6 Li3 0.00(9) 1_455 1_455
Mo2 O6 Co3 122.34(9) . 6_556
Co3 O6 Co3 91.35(7) 1_455 6_556
Zn3 O6 Co3 91.35(7) 1_455 6_556
Li3 O6 Co3 91.35(7) 1_455 6_556
Mo2 O6 Li3 122.34(9) . 6_556
Co3 O6 Li3 91.35(7) 1_455 6_556
Zn3 O6 Li3 91.35(7) 1_455 6_556
Li3 O6 Li3 91.35(7) 1_455 6_556
Co3 O6 Li3 0.00(6) 6_556 6_556
Mo2 O6 Zn3 122.34(9) . 6_556
Co3 O6 Zn3 91.35(7) 1_455 6_556
Zn3 O6 Zn3 91.35(7) 1_455 6_556
Li3 O6 Zn3 91.35(7) 1_455 6_556
Co3 O6 Zn3 0.00(6) 6_556 6_556
Li3 O6 Zn3 0.00(6) 6_556 6_556
Mo2 O7 Zn2 155.72(9) . .
Mo2 O7 Co2 128.79(9) . 6_556
Zn2 O7 Co2 75.48(5) . 6_556
Mo2 O7 Zn2 128.79(9) . 6_556
Zn2 O7 Zn2 75.48(5) . 6_556
Co2 O7 Zn2 0.00(3) 6_556 6_556
Mo2 O7 Li2 128.79(9) . 6_556
Zn2 O7 Li2 75.48(5) . 6_556
Co2 O7 Li2 0.00(3) 6_556 6_556
Zn2 O7 Li2 0.00(3) 6_556 6_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O1 1.753(2) .
Mo1 O2 1.7686(15) 7_565
Mo1 O2 1.7686(15) .
Mo1 O3 1.811(2) .
Mo1 Li1 3.3480(6) 7_565
Mo2 O6 1.7532(15) .
Mo2 O7 1.7624(15) .
Mo2 O4 1.7862(15) .
Mo2 O5 1.7868(14) .
Zn1 O4 2.0415(14) .
Zn1 O5 2.0784(15) 1_655
Zn1 O3 2.0876(11) .
Zn1 O2 2.0996(14) 1_455
Zn1 O5 2.1375(15) 5_656
Zn1 O2 2.2269(16) 5_756
Zn1 Li1 3.1521(8) 5_756
Zn1 Zn1 3.1521(8) 5_756
Zn1 Li1 3.2214(8) 5_656
Zn2 O7 2.0716(17) .
Zn2 O7 2.0716(17) 7
Zn2 O7 2.0839(17) 6_656
Zn2 O7 2.0839(17) 4_545
Zn2 O1 2.136(2) 2_654
Zn2 O1 2.145(2) 5_756
Zn2 Zn2 2.5436(5) 6_656
Zn2 Co2 2.5436(5) 6_656
Zn2 Li2 2.5436(5) 6_656
Zn2 Li2 2.5436(5) 6_556
Zn2 Co2 2.5436(5) 6_556
Zn2 Zn2 2.5436(5) 6_556
Zn3 O4 2.1158(18) .
Zn3 O4 2.1158(18) 7_565
Zn3 O6 2.1705(19) 7_665
Zn3 O6 2.1705(19) 1_655
Zn3 O6 2.2264(19) 6_656
Zn3 O6 2.2264(19) 4
Zn3 Zn3 3.1457(19) 6_556
Zn3 Li3 3.1457(19) 6_556
Zn3 Li3 3.1457(19) 6_656
Zn3 Zn3 3.1457(19) 6_656
O1 Co2 2.136(2) 2_655
O1 Li2 2.136(2) 2_655
O1 Zn2 2.136(2) 2_655
O1 Zn2 2.145(2) 5_756
O1 Li2 2.145(2) 5_756
O1 Co2 2.145(2) 5_756
O2 Co1 2.0996(14) 1_655
O2 Zn1 2.0996(14) 1_655
O2 Li1 2.0996(14) 1_655
O2 Co1 2.2269(15) 5_756
O2 Li1 2.2269(15) 5_756
O2 Zn1 2.2269(15) 5_756
O3 Co1 2.0876(11) 7_565
O3 Zn1 2.0876(11) 7_565
O3 Li1 2.0876(11) 7_565
O5 Co1 2.0784(15) 1_455
O5 Zn1 2.0784(15) 1_455
O5 Li1 2.0784(15) 1_455
O5 Co1 2.1376(14) 5_656
O5 Li1 2.1376(14) 5_656
O5 Zn1 2.1376(14) 5_656
O6 Co3 2.1705(19) 1_455
O6 Zn3 2.1705(19) 1_455
O6 Li3 2.1705(19) 1_455
O6 Co3 2.2264(19) 6_556
O6 Li3 2.2264(19) 6_556
O6 Zn3 2.2264(19) 6_556
O7 Co2 2.0839(17) 6_556
O7 Zn2 2.0839(17) 6_556
O7 Li2 2.0839(17) 6_556
